1 DISTORTIONOF BASE PLATE DENTURES AS A FUNCTION OF THEIR THICKNESS ANTONIO JOAQUIM PELLIZZER * DIORACY FONTERRADA VIEIRA ** PELLIZZER, A. J. & VIEIRA, D. F. - Distortion of base plate dentures as a function of their thickness. Rev. Odont. UNESP, 8/9:81-89, 1979/1980. SUMMARY: The misfit of denture bases was evaluated. Three different :acry Ue resins were employed: heat curing, self-curing and "fluid" resins. The denture bases were measured after their release of the casts and storage in 37 C distilled water durillg 7 days. Bach kind of acrylic resin had a different behavior as related tot its thickness and storage in distilled watter, being the self-curing type that presented the less misfit. KEY WORDS: Denture base, acrylic resin, dimensional changes. Dimensional changes of the acrylic resin denture base do occur during its processing and are causes of distortion and lack af its adaptation to the soft tissues, what is mostly evidenced in the posterior part of the palate. Polymerization shrinkage and its partial inhibition by the the stone matrix are the causes of the distortion. Self-curing acrylic resin molded by the flow of "fluid resin" are said to adapt be-tter than the heat curing one to the stone working model (SHE PARD, 1968); but there are those who think the former distort more during processing than self-curing and heatcuring acrylic resins molded under compression (GOODKING & SCHUL TE, 1970; KRAUT, 1971). It has been shown also that the distortion of seucuring fluid resins may be due to the differences in thickness, and that thin base dentures present twice as much shrinkage than the thicker ones (WINKLER et al., 1971a; WINKLER et al., 1971b). The lack of complete agreement in regard to the influence of the three types of acrylic resins (selfcuring and heat curing molded by compression, and self-curing molded by pouring it in a flexible matrix) and thickness on the distortion of denture bases, suggested the present '" *'" Disciplina de Prótese. Faculdade de Odontologia de Araçatuba, UNE8P, São Paulo, Brasil. Departamento de Materiais Odontológicos. Faculdade de Odontologia de São Paulo, USP, São Paulo, Brasil. 81
2 82 PELLIZZER and VIEIRA Rev. Odont. UNESP 1979/ vol. 8/9 study. Its purpose- it to observe the effect of several factors on the denture base distortions. \ MateriaIs a~d Methods One self-curing acrylic resin tray (Clássico, Artigos Odontológicos Clássico) was obtained for the metal madel (Fig. 1); the space betwe-en the master model and the acrylic resin tray was uniform and its thickness. was 2.5 mm. Stone models, replicas of lhe metal master model, were obtained with the acrylic resin tray, a polyesther impression material (Impregnum Espe., Western Germany) and stone (BR Produtos Dentários BR) through a conventional technic. Wax base plate-s (n. o 7, in sheets, Indústria e Comércio de Artigos Dentários) were obtained on the stone models; their lower borders were 5mm far from the lower border of the stone model anterior and lateral walls; the posterior lateral wall of the model was left free. Thickness of the wax base plates. were: a) 3.0 mm uniformly thick, b) 1.0 mm uniformly thin, c) thick in the alveolar ridge and thin in palate region and d) thin in the alveolar ridge and thick in the palate region. Reference points for the places where measurements would be performed were marked in 3 points for the micrometer microscope (right and left alveolar ridge for the posterior region and a central point in the posterior region of palate) and in 7 points for the diai gage measurements; these points and the wax base plate thinckness were kept constant in all the wax base plate-s, through one stone index or matrix made in three parts, as shown in figure 2. The wax base piates we re invested in stone contained in a flask, for the self-curing and the heat-curing acrylic resins (Clássico, Artigos Odontológicos Clássico) molded under compression; the self-curing "~h~id" ac~ylic resin (Artigos OdontologlCos Classico) was invested in the irreversible hydrocolloid provided with the sarne. After the removal of the wax base plate from the investing ~aterial. and the lining of the later,with an lnsulating mate-rial the acrylic resins. doughs were molded according to their manufacturer; polymerization was perfomed according to a conventional cycle (TUCKFIELD et al., 1943) for the heat-curing resin at room temperature for the s3lf-curing one and at 50 C, in humid athmosphe re, under a preassure of 22 pounds, in special equipment (Class-Press, Artigos Odontológicos Clássico). After deflasking the base plate dentures they were just finished, but not polished and the measurements were performed. The spaces between the acrylic resin base plate denture were measured with the equipments already mentioned when it was used the dial gage the metal master model was horizontally located, under it; the first n1easurement was done with the base plate denture in position and the second of the model alone without the base plate denture; the space between was then calculated. With the micrometer microscope, there were measured, directly, the distances from the acrylic resin base plate denture and the model, at the three nlentioned points. Over those experimental factors described (three of resin and thikness of base plate), we have made the measurements in 3 different times: immediately after deflasking the polymerized base plate denture, 7 days
3 THICKNESS AND DISTDRTIDN DF BASE PLATE DENTURES 83 after its immersion in distilled water at37 C, ande before the removai of the base piate from its mode!. Those conditions correspond to a factorial desi~3x4x2 = 24 from which the tinles of measurements are fictitious, because they were performed in the sarne denture. We had then 12 different experimental conditions; there were made 10 sampies (dentures) for each experimental condition a total of. 120 base plate dentures; for three times of measurement we had 360 serie of measurements; and for two different misfit determinations (before and after the water immersion) there were 720 series of measurements of misfit. These determinations were performed for three points of each denture with the micrometer microscope (a total of 720 measurements) and for 7 points of each denture with the dail gage (1680 measurements). Analysis of variance of the "splitplot" type were performed for the results obtained with the micrometer microscope and with the diai gage; when judged convenient there were calculated the means and criticai values of significant factors and interactions. Results There wili be reported here only the results for micrometer microscope because are similar to those for the dial gage. The analysis of variance for the micrometer microscope values indicated that in regard to the base plate dentures misfit the materiais used behaved differently, but not their thickness; the points where the measurements were performed did present different misfits; the phases of meas.- urements did present different results; and several interactions were statistically different. Table 1 presents the misfit means for each levei of the principal factors studied, as well as the criticai value for those with more than two leveis. lt is seen that self-curing acrylic resin presented smaller misfits than the heatcuring and the "fluid resin" ones. The different thickness did present diverse misfits, althoug it is seen that the dentures with unifonn 3.0mm thickness did present less misfit than the other thickness. ln regard to the points or regions of measurements, it is clear that the misfit is not uniform, but different in these points which means that the denture suffers an overall distortion as a consequence of the partially inhibited polymerization d.imen~üonal changes; this is due t.o the induced stress and the later posliberation. As it should be expected the water immersion, time (7 day storing) and temperature (37 C) did contribute to a greater distortion and misfit of the dentures, as shown in the last line of table 1. vve could find a s.tatistically significant interation between acrylic resin types and base plate dentures thickness, with a criticall valüe of 27.5, significant at the 5% levei. It confirms the observed fact that the self-curing acrylic resin does present less general distortion than the heatcured one and that the self-curing "fluid" resin; heterogeneous thickness tend to cause greater misfits than homogeneous one. Uniformly thin (1.0 mm) acrylic resin dentures tended to present the greatest misfit. A significant interaction was aiso found between acrylic resin types and regions. of measurements (criticai value was 13.4 at 5% levei of significancy). The important observation is
4 84 PELLIZZER and VIEIRA Rev. Odont. UNESP 1979/ vol. 8/9 TABLE 1 - Average misfits (um of the base piate dentures, as a,function of acrylic resin type, thickness, regions of measurement, time of measurement, and criticai value for differences between each two means. Acrylic Resin Tukey heat-curing seif-curing "FIuid" self-curing (5%) ,8* Denture thickness Uniform Heterogenous 1.0mm 3.0mm PaIatine vauit FIanges 1.0mm 3.0mm PaIatine vault Flanges 3.mm l.mm Regions of measurement right posterior posterior of palate Ieft posterior ,8* Time of measurement Before immersion in water after 7 days immersion in 370C water s * - statistically significant, "':3: _ not significant
5 THICKNESS AND DISTO RTION OF BASE PLATE DENTURES 85 that the self-curing base plate dentures presented similar misfits in the three different regions of measurements, while heat-curing and "fluidresin" presented different values for those regions meaning that the later two distorted more than the former. The interaction between base denture thickness and regians af measurement confirms that the uniformly thicker (3. Omm)dentures distorted less and presented smaller misfits than the uniformly thin and the he-terogeneous base plate dentures (1 % significant criticai value=16.3) Average misfits for the interaction betw -en resins and time of measurements confirms once more that storage, temperature (37<>C) and water immersion increase the misfists; however, the misfits due to them only accurred for heat-cured and "fluid" resins. Average misfits for the interaction between base plate denture thickness and time shown that uniformly 3. O mm thick denture tends to present smaller misfit than the uniformly 1.O mm thick and the heterogeoulsy thick ones, as a cansequence of storage in 37 C water (1 % significant criticai value = 7.8). The data obtained with the diai gage, when statistically evaluated through an analysis of variance. presented results similar to thos.e obtained with the micrometer micrascope. A statistical comparison between the results obtained with these instruments showed that the micrometer microscope made it possible to obtain results numerically greater than those found with the dial gage; this may mean a greater possibility af finding differences between two means when using the micrometer microscope to read the distance between the points of measurement. Discussion Our results confirm in a general pattern what is generally known in regard to the base plate denture, as pointed by previous researchers (GOODKING & SCHULTE, 1970; KRAUT, 1971; WINKLER et al., 1971; 'VOELFEL et al., 1959; WOELFEL et al., 1961; WOELFEL et al., 1962, WOELFEL et al., 1965). Under the practical standpoint it is interesting to stress that there is a general tendency for the base plate acrylic resin dentures to present an he-terogeneous misfit, in regard to its model; this heterogeneous mislfit is consequent to dimensional changes that the acrylic resin suffers during the dental laboj'atory polymerization processo The higher the dimmensional changes, the higher the induced stresses and thus the- greater the distortion and misfit between the denture and its master mlqdel; it is for this reason that the "self-curing' acrylic resin, which dimensional change is smaller than that of the heat-curing one (WOELFEL et al., 1959; WOELFEL et al., 1960; WOELFEL et al., 1961; WOELFEL et al., 1962; WOELFEL et al., 1965) presents less misfit than the later. For this reason it was a surprise to see that the "fluid" resin presented greater misfit than the "self-curing" one, which is possibly due to a camposition factor and also to its particular processing technic; this result do agree, howe'ver, with previous statements (GOODKING & SCHULTE, 1970; KRAUT, 1971). Thin base plate dentures tend to present greater distortions and thus
6 86 PELLIZZER and VIEIRA Rev. Odont. UNESP 1979/ vol. 8/9 greater misfit, as already stressed in the literature (HARMAN, 1949). During the aerylie resins denture bases proeessing there are indueed stresses whieh are C:ifficult to release, due to the strenght of the solid eured aerylic resin; it is for this reason that those faetors whieh make easier the stress release (storage, water immersion, high te mperature) tend to inerease distortion and misfit. These observations and the interaetions bet:ween the levei of the faetors studied are of use to those' which proeess and provide base plate dentures to patients, and are helpfull to interpret the changes observed in their proeessing. Summary and ConcIusions Base plate dentures were proeessed using three different types of aery Ue resins: heat-euring, self-euring, and "fluid" self-euring ones. These dentures were obtained in four thiekness. which were different in the following way: uniformly thiek (3. Omm) or thin (1. Omm), heterogeneously thiek (3. O mm i11 the palatine vauit and 1. Omm in the flanges, or 1. Omm in the palatine vault and 3. Omm in the flanges). These dentures. were processed accord- ing to the respe'ctive aerylic resins manufacturers. After proeessing and deflasking they were measured in determined points of each denture, to evaluate the misfit between them and the respeetive model, after their release of the eorre~lpondentmode ls and after storage of the data obtained made it possible to arrive to the following eonelusions: 1) the three types of acrylie resins behaved differentiy in regard to the observed misfit, the selfeuring type prese-nting smaller misfits than the heat-euring and the "fluid resin" ones; 2) there was a tendency for the uniformly thiek (3.0mm) dentures to present smaler misfit than the uniformly thin (1.0mm) ànd the heterogenously thick ones; 3) the observed misfit was not equal in the various regions where it was measured; it was greater in the posterior re'gions of the denture and smaller in the anterior region; this differenee does eorrespond to a general distortion of the denture; 4) the misfits observed tends to increase with the seven days storage of the dentures in 37 C distilled water and a statistically signifieant difference was found for the data obtained with micrometer mieroscope and dial gage, the former presenting larger misfit results than the later.
7 THICKNESS AND DISTDRTIDN DF BASE PLATE DENTURES 87, PELLIZZER, A. J. & VIEIRA, D. F. - Distorção da base de dentadura em função de sua espessura. Rev. Odont. UNESP, 8/9:81-89, 1979/1980. Foram confeccionadas bases de dentaduras usando três tipos diferentes de resinas acrílicas: de ativação térmica, de ativação química, e de ativação química "fluida". Estas dentaduras foram obtidas em quatro espessuras diferentes: espessura uniforme (3mm) ou fina (lmm), espessura heterogênea (3mm no palato e lmm nos rebordos, ou lmm no palato e 3mm nos rebordos}. Estas dentaduras foram obtidas de acordo com as instruções dos fabricantes. Após a polimerização e desmoldagem elas foram medidas em pontos determinados, para avaliar o desajuste entre elas e o respectivo modelo, após a sua separação do modelo e após a imersão em água destilada a 370C por 7 dias. A avaliaç;ão estatística dos dado;:; obtidos possibilitaram concluir que: 1) os três tipos de resinas acrílicas sle comportam diferentemente em relação ao desajuste, o tipo ativado quimicamente apresentou menores desajustes do que os tipos ativado termicamente e ativado qui micamente "fluido"; 2) houve uma tendência para um desajuste menor nas den taduras uniformemente espessas (3mm) em relação:a uniformemente fina (lmm) e as de espessuras heterogêneas; 3} o desajuste observado não é igual nas vária~ regiões medidas; é maior na região posterior e menor na região anterior; estas diferenças correspondem a uma distorção geral das dentadur.as; 4)1 os desajustes observados tendem a aumentar após a imersão em água destilada a 370C durante 7 dias; 5) foi constatada diferença estatística significante entre os dados de desajustes obtidos com o relógio micrométrico e o microscópico comparador, sendo maiores as medidas de desajuste neste último. Acknowledgements The authors are thankful1 to Prof. Antonio Muench for the statistical analysjs. REFERENCES GOODKING, R.J. & SCHULTE, R.C Dimensional accuracy of pour acrylic resin and conventional processing of cold-curing acrylic resin bases. J. prasth. Dent., 24: HARMAN, I. M Effects of time and temperature on polymerization of a methacrylate resin denture base. J. Amer. dent o Ass., 38: KRAUT, Ro Ao A comparison af denture base accuracy. J. Amer. dento Ass., 83:353-7 o SHERPARD, Wo L Denture bases processed from a fluid resin. J. prasth. Dent., 19: TUCKFIELD, WoJ.; WORNER, H.K. & GUERIN, B.Do Acrylic resins in dentistry. Part I, Austral. J. Dent., 45:1-25. WINKLER, S.; ORTMAN, HoR.; MOR RIS, H. F. & PLEZIA, R. A. 1971a. Pracessing changes in complete dentures canstructed from pour resins. J. Amero dent. Ass., 82: WINKLER, S.; ORTMAN, H. R; MOR RIS, H. F. & PLEZIA, R. A. 1971b. Investing mediuns for pour re5ins J. Amer. dent., 83: WOELFEL, JoB., PAFFENBARGER, G. C. & SWEENEY, W.T Dimensional accuracy of denture base resins. J. dento Res., 38:752.
8 88 PELLIZZER and VIEIRA WüELFEL, J.B., PAFFENBARGER, G. C. & SWEENEY, W. T Dimensional changes occuring in dentures during processing. J. Amer. dento Ass., 61: WüELFEL, J.B., PAFFENBARGER, G. C. & SWEENEY, W. T Changes in dentures during in water and in service. J. Amer. dento Ass., 62:643.~7. Rev. Odont. UNESP 1979/ vol. 8/9 WüELFEL, J.B., PAFFENBARGER, G, C. & SWEENEY, W. T Dimensional changes in complete dentures on drying, wetting and heating in water. J. Amer. dento Ass. 65: Recebido para publicação em LEGENDS Fig. 1. StainIess steei master model Fig. 2. Stone index to controi thickness of wax base plate dentures and to determine the points for misfit measurements.